Free-electron response in reflectance anisotropy spectra
K. Fleischer,1,2,*S. Chandola,1,2Th. Herrmann,2 N. Esser,3 W. Richter,2,4and J. F. McGilp1 1School of Physics, Trinity College Dublin, Dublin 2, Ireland
2Technische Universität Berlin, Institut für Festkörperphysik, Sekr. PN 6-1, Hardenbergstrasse 36, D-10623 Berlin, Germany 3ISAS-Institute for Analytical Sciences, Department Berlin, Albert-Einstein Strasse 9, 12489 Berlin, Germany
4INFM, Universitá di Roma Tor Vergata, Via della Ricerca Scientifica 1, I-00133 Roma, Italy 共Received 28 March 2006; revised manuscript received 3 October 2006; published 27 November 2006兲 Reflectance anisotropy spectra共RAS兲, extended into the near infrared spectral region, of anisotropic metal islands, metal surfaces, and atomic nanowires are analyzed with respect to anisotropies in the optical response of the free-electron gas of such low dimensional metal structures. In order to distinguish conductivity and morphology effects, both a phenomenological anisotropic Drude model and an effective medium model using ellipsoidal metal inclusions are used to model the spectra. In some cases共metal islands兲the RAS response is dominated by the free-electron contribution, while this contribution is significantly smaller for the metal surfaces and nanowires in the accessible spectral range.
DOI:10.1103/PhysRevB.74.195432 PACS number共s兲: 73.50.⫺h, 73.20.At, 73.63.Nm, 73.25.⫹i
In this work the contribution of the free-electron gas to the reflectance anisotropy spectra共RAS兲of low dimensional metallic nanostructures or nanowires will be addressed. In-terest in such metallic nanowires and their basic properties has increased in recent years, particularly for wires on sur-faces with widths of a few atoms. These can show interesting effects such as Peierls instabilities and charge density waves
共CDW兲, and are also promising candidates for investigating more exotic effects such as spin charge separation.1–4So far, investigations have been mainly performed using electron based methods such as scanning tunnelling microscopy and spectroscopy共STM, STS兲, and angle resolved photoemission spectroscopy共ARPES兲. Due to the limited penetration depth of electrons, these methods are highly surface sensitive but are only suited for nanostructures on surfaces, or the surfaces themselves. This is a problem for characterizing metallic nanowires in devices, since the properties of the wire need to be known even if they are buried below protective caps to ensure stability in ambient conditions. One possible way to overcome this limitation is to use surface or interface sensi-tive optical probes, as the larger penetration depth of light allows buried structures to be accessed.
One prominent optical technique with such surface and interface sensitivity is reflectance anisotropy spectroscopy
共RAS兲. The technique itself was introduced in the mid 1980s5–7and is nowadays used in both surface science and in semiconductor technology关as growth control in gaseous en-vironments, such as in metal organic vapor phase epitaxy
共MOVPE兲, where electron based methods cannot be applied8,9兴. The origin of the RAS response from anisotropic surfaces is quite well understood and can be calculated ab initiowithin density functional based theories.10,11The main structures in the RAS spectra arise from transitions between surface states or surface modified bulk states. RAS is well suited for the analysis of metallic nanowires and has proved to be a useful tool in monitoring nanowire formation12,13or Peierls driven metal-insulator transitions in metallic nanowires.14 For such systems the spectral signature of the
interband electronic transitions has already been discussed.15 In contrast to these earlier studies, this paper focuses on the intraband transitions and the direct observation of a con-ductance anisotropy with RAS. Experimentally the basic idea is to observe these contributions in the near infrared共IR兲 spectral region, similar as it has been done for the free-carrier contribution to the dielectric function 共absorption兲, where the intraband contributions start to dominate.16,17 It will be shown that this response can be modeled by using a Drude-type dielectric function with two independent tensor components,˜xand˜y, contributing to the anisotropic RAS signal. This simple model appears promising in relating the measured spectra of metallic nanowires to the conductance anisotropy, thus facilitating contactless measurements of this quantity. Theoretical ab initio calculations of the interband anisotropy from the 共110兲-surface of Cu and Al 共Ref. 18兲 already indicate that such contributions to the reflectance an-isotropy exist.
II. DETAILS OF THE OPTICAL MODELS
RAS measures the difference in the reflectance of light polarized along two orthogonal axes xand yin the surface plane, normalized to the mean reflectance.
⌬R R = 2
If the complex Fresnel reflection coefficient, ˜r, can be measured, then
⌬˜r r ˜ = 2
As the anisotropy is normally small, ⌬R/R⬇2 Re共⌬˜r/˜r兲. Both⌬R/Rand Re共⌬˜r/˜r兲have been termed RAS signals in the literature:7here only the latter will be used.
A. The surface dielectric anisotropy
compared with calculations within a three layer model,19 comprising an isotropic bulk with dielectric function˜b, a modeled effective anisotropic layer for the nanowires
共˜x,˜y兲, and finally air as the ambient layer. The RAS can then be expressed as
⌬˜r r ˜ =
whered is the effective thickness of the anisotropic layer.5 The quantityd共˜x−˜y兲 is called the surface dielectric aniso-tropy共SDA兲and is a robust quantity: in the absence of other information, the division betweendand共˜x−˜y兲is uncertain. With Eq.共3兲it is possible to calculate the RAS spectra using model dielectric functions for comparison with experiment or, since ˜b is usually known, to discuss RAS spectra in terms of the dielectric anisotropy by calculating the SDA from the measured spectra.
For the measurements presented here, the three layer de-scription is sufficient. In the case of buried structures more complex models have to be used: for example, the dielectric anisotropy of the surface and interface have been success-fully separated for AlAs/ GaAs heterostructures.20In this ini-tial study only uncapped wires are analyzed and the simple three layer model is sufficient.
Frequently RAS spectra show structure close to bulk criti-cal points of the substrate which partly originate from the normalization by˜bin Eq.共3兲and partly by interface modi-fied bulk states. To distinguish these from the response of the nanowires the bulk critical points are marked in all figures, e.g.,E1,E1+⌬1,E0
⬘, and E2 in Fig.3.
B. Model dielectric functions
In order to describe the dielectric function of the metallic nanowire two different approaches will be compared. The first utilizes a three-dimensional共3D兲-Bruggemann effective medium approximation共EMA兲assuming an ellipsoid shape of the wire. The anisotropic layer is then described by a modified, anisotropic Bruggeman EMA, using a mixture of the ellipsoids of bulk metal dielectric function and vacuum.21 The percolation threshold is f= 1 / 3 for spherical inclusions in this model although, in its anisotropic formulation using ellipsoids, f itself is anisotropic, with larger values in the direction of the long axis of the ellipsoid and smaller values along the short axis.21This approach has been used success-fully for modeling the effect of roughness on RAS spectra of clean semiconductor surfaces.22 As will be seen later, this approach works well for larger anisotropic islands, but fails to describe the case for wires with diameters smaller than 50 nm. Instead a simpler, phenomenological approach can be used, where only anisotropy in the free-electron properties are assumed.
The dielectric function of a free-electron gas can be de-scribed using the Drude-Lorentz formulas for an oscillator with eigenfrequency0= 0:
⬘= 1 − p 2
⬙. In these formulas␥共=1 /兲is the scattering rate which is related to damping with a phenomenological scattering time of . In the Drude theory, p is given by
p2=Nce2/共me0兲 where Nc is the free-electron density and
me the free-electron mass. Although originally derived for noninteracting electrons in 3D, the Drude dielectric function nevertheless agrees well with the measured dielectric function of bulk metals.23–26
The optical anisotropy in a free-electron gas may thus be caused by anisotropic values of the effective masses共 replac-ing the free-electron mass兲and/or scattering rates. As a first approximation, the experimental bulk plasma frequency is used 共implying an isotropic effective mass兲, while different values for the scattering rate are assumed here for the two orthogonal directions probed with the RAS. This seems rea-sonable, as scattering in metals at room temperature is a nanoscale phenomenon, allowing surface and interface scat-tering from anisotropic nanoscale structures to produce an-isotropic scattering rates. This will be discussed further in Sec. VII. The set of parameters共p,␥x,␥y兲appears sufficient to describe the infrared SDA. For RAS model calculations, the thickness of the layerdis needed as an additional param-eter. Figure1shows an example of a model RAS calculation of such an anisotropic Drude layer on silicon, where the effect of varying the anisotropic scattering rate is shown.
Such a contribution to the RAS of metallic structures has been discussed but, due to the limited spectral response of most RAS systems, the contribution was always found to be too weak for quantitative analysis.27–29 As will be shown here, metallic nanowires on semiconductor surfaces can
pro-FIG. 1. Model RAS spectra of an anisotropic Drude layer on silicon. The solid line shows a calculation with an anisotropy ␥y/␥x= 1.2, the dashed line one with␥y/␥x= 2. The anisotropic
duce a stronger response, particularly in the energy region below 1 eV, which is accessible with the IR enhanced RAS spectrometer described below.
C. Anisotropic conductivity
As the IR reflectance anisotropy of a 1D metallic system can be related to a free-electron contribution, the question arises whether conclusions about the conductivity can be drawn from RAS spectra as well. The dielectric function is related to the optical conductivity,˜:19,30
˜= 1 −i˜/0. 共5兲 The RAS signal can be described in terms of a conductivity anisotropy,⌬˜=˜x−˜y, by using this relation and the three layer model of the RAS signal from Eq.共3兲:
⌬˜r r ˜ =
Hence the RAS signal is directly proportional to this conduc-tivity difference. The RAS spectra allowsd⌬˜ to be deter-mined, analogously to the SDA. This is particularly useful, asd⌬˜ is the anisotropy in the sheet conductance determined by conventional four-point electrical measurements, assum-ing the underlyassum-ing bulk does not contribute significantly. Fit-ting the infrared RAS using the anisotropic Drude model allows⌬˜ to be determined at zero frequency, thus giving an estimate of the dc conductivity. Such a calculation corre-sponds to an extrapolation of a measured ac conductivity to = 0. Infrared transmittance spectroscopy has been used previously to determine the conductivity of 2D films:31,32it is shown here that IR enhanced RAS is sensitive to the conductivity anisotropy of 1D structures.
The RAS instruments follow the basic design of a two polarizer system and photoelastic modulator共PEM兲, as pro-posed by Aspnes et al.7 One broad range RAS system
共0.75– 6.5 eV兲 and one IR optimized system 共0.5– 4.5 eV兲 were used for the measurements presented here. Both sys-tems utilize multiple detectors: InGaAs/ Si diodes and pho-tomultiplier in the first case, and a combination of liquid nitrogen cooled InAs photodiode and InGaAs/ Si diodes in the latter case. In order to access such a broad spectral range, both systems were equipped with either two independent monochromators or a double grating monochromator. All op-tical components were chosen for broad range performance with, for example, MgF2 polarizers and CaF2 PEMs being used. A Xe arc discharge lamp was normally used, although for some IR measurements this was replaced by a quartz halogen lamp, although this limits the range to 0.5– 3.0 eV. The sample preparation was always performed under ultrahigh vacuum conditions at a base pressure below 1⫻10−10mbar. The InAs共110兲surfaces were prepared byin
situcleavage, the Si共111兲by removing the native oxide layer at 1100 ° C. The metal surfaces were cleaned by sputter and annealing cycles. For the preparation of the Sn and In nano-wires, the metals were deposited onto the clean surfaces from
Knudsen-type evaporator cells. In the case of Sn/ InAs共110兲, the deposition was performed at room temperature and was controlled with a quartz microbalance, calibrated using Au-ger electron spectroscopy 共AES兲 and ex situ atomic force microscopy 共AFM兲 measurements of the average island height. In the case of the In/ Si共111兲 system the sample was kept at 450 ° C during the indium deposition and the forma-tion of the indium nanowires was monitored directly by the RAS measurement. The presence of the single domain
共4⫻1兲 reconstruction of surface was checked afterwards with low energy electron diffraction共LEED兲.
IV. ANISOTROPIC METAL ISLANDS
Two systems of metallic nanostructures are discussed here. Anisotropic islands of ␤-tin grow on InAs共110兲, and produce large infrared RAS structures. The second system, which also grows anisotropic metal islands, is Pb/ Si共335兲, which was investigated by Stròżaket al.with another optical technique, surface difference spectroscopy共SDR兲.33This in-teresting work includes sufficient polarization dependent measurements to enable a RAS response to be calculated from the data, for comparison with the anisotropic Drude model.
A. Sn/ InAs„110…
Anisotropic islands of ␤-tin were grown on cleaved InAs共110兲 surfaces at room temperature. In Fig. 2 atomic force micrographs, taken ex situ, are shown for nominal thicknesses of 20 and 100 ML of Sn. The islands become more isotropic as the coverage increases. By 100 ML, large rectangular islands of␤-tin have been formed. Although the exact crystallographic orientation is not known, the shape anisotropy of the islands suggest that the tetragonalc-axis is within the surface plane.
In Fig.3the RAS spectra of a 40 and a 60 ML sample are shown. The spectra are dominated by the bulk Sn response, although there is still some structure in the region of the bulk critical points of the InAs substrate共labeled兲, which are ma-jor features in the RAS spectra at very low coverages. The spectra can be qualitatively understood by an anisotropic
3D-FIG. 2. AFM images of共a兲 20 ML and共b兲100 ML of Sn on InAs共110兲. For smaller coverages the tin islands are highly aniso-tropic with a long axis of up to 400 nm and a short axis of only 25 nm. At higher coverages the islands are larger but more isotropic
Bruggeman effective medium approximation 共EMA兲 with oriented ellipsoidal inclusions21,22 of bulk Sn, as shown by the dashed curve in Fig. 3 共d= 3 nm, x= 250 nm,
y= 100 nm, f= 0.5, where f is the filling fraction兲. The effec-tive dielectric function is individually calculated for light polarized along, and perpendicular to, the long axis共˜x,˜y兲. The AFM images were used to determine values forxandy, while the thickness,d, in Eq. 共3兲 was fitted to obtain best agreement with the measurement. It is clear that this approxi-mation fails to describe the strong IR increase occurring at lower coverage, but provides qualitative agreement with the general line shape of the 60 ML spectra. The agreement is reasonable, considering that the bulk dielectric function used in these calculation was derived from microcrystalline samples with random orientation.34 The islands here are clearly oriented, and the much sharper structure around 1 eV in the measured RAS response probably arises from an an-isotropic absorption in the tin, which is broadened in the measured˜b,Snof the randomly oriented crystals. Addition-ally, a strong broad minimum in the 3 – 5 eV region evolves for higher coverages which is part of a Mie resonance occur-ring for large islands. Such structures were already seen and successfully simulated for larger indium islands on GaAs.35 In the case of the 60 ML sample a fit using the anisotropic Drude model does not provide any new information. Although it does agree well in the IR when the areas of strong interband transition are excluded, the simple mor-phological model using the bulk Sn dielectric function and an anisotropic EMA provides equally good agreement.
For smaller coverages共⬍40 ML兲, where the anisotropies in the island geometry are much more pronounced, the EMA model is not sufficient to reproduce the RAS line shape
共see inset Fig. 4兲. In particular, the strong signal in the IR
regime cannot be explained, while the simpler Drude model reproduces the results very well.
The IR structure emerges for coverages above 1.5 ML and shows a peak at 1.3 eV that redshifts with increasing cover-age共0.8 eV at 7 ML; 0.6 eV at 14 ML兲. This behavior could arise from a number of factors. First, changes in gradient in the IR tail of the two orthogonal polarizations may produce a peak when the difference is plotted. Second, if the metallic layer is above the percolation threshold, the Drude-like di-electric response may not increase monotonically to lower energies.32,36 Third, EMA models using elliptical inclusions produce a percolation threshold that depends on the elliptic-ity, which changes significantly with coverage共see Fig. 2兲. Detailedin situ studies of the morphology in this coverage regime would be necessary to clarify the importance of these various contributions.
For higher coverages共⬎14 ML兲the IR response at 0.8 eV is maximal at 25 ML and then decreases until the morpho-logical anisotropy dominates the spectra above 40 ML, as discussed above. The quality of agreement achieved with the anisotropic Drude model is shown for a 20 ML sample in the inset of Fig.4. Least-square fits of model parameters in this coverage region give sufficiently good agreement that quan-titative information can be extracted from the RAS spectra. The number of free parameters is minimized by using known values where possible. The thickness,d, was set to the nomi-nal layer thickness, andpwas set to the␤-tin bulk value of 13 eV.34The remaining two parameters共␥x,␥
y兲were deter-mined by least-squares fits of the SDA共see Fig.5兲. The best agreement is obtained in the range 10–30 ML. In TableIthe results are summarized and an estimation of the anisotropy in the dc conductivity is given by extrapolating the Drude-like RAS response to zero frequency. It is important to note that these predictions can only account for the free-electron
con-FIG. 3. RAS spectra of 40 ML共gray line兲 and 60 ML共black line兲coverage of Sn. The general line shape of the 60 ML sample can be modeled using the bulk properties of Sn and an anisotropic effective media approximation共dashed line兲. The strong infrared RAS signal in the 40 ML spectrum共and at lower coverages兲cannot be explained with such effective medium models. For comparison a least-squares fit using the anisotropic Drude model is also shown. The regions with strong Sn interband contributions were excluded in the fit.
tribution to the conductance and also neglect any percolation effects.
TableIshows that, as expected, the scattering rate is uni-formly higher in the shorter,ydirection of the anisotropic Sn islands. Also, the values of the anisotropy in the sheet con-ductance appear reasonable. The sheet concon-ductance, esti-mated using the bulk conductivity of tin and the layer thick-ness for the 20 ML sample, gives 32⫻10−3 S /䊐, while the measured anisotropy in the conductance is 2.3⫻10−3± 0.5 ⫻10−3S /䊐. The fractional anisotropy of 0.04 is a lower limit because the conductivity of such a thin granular film is expected to be significantly lower than the bulk value.37For example, if the measured values for Sn layers共⬎5 nm兲 on glass38 are extrapolated to the thickness of the 20 ML sample, a value ofdof 6⫻10−3S /䊐is obtained, giving a fractional anisotropy of 0.38. The values ford⌬in TableI, which vary from 0.2⫻10−3to 2.3⫻10−3 S /䊐, are clearly reasonable.
It should be noted that the fitted value obtained for the anisotropic sheet conductance is relatively robust to param-eter changes. For example, ifpis set to the surface plasmon frequency p,s=p,b/
冑2, equally good fits can be derived, which have smaller scattering rates but larger anisotropies: for the 20 ML sample,␥x= 0.93 eV and␥y= 2.1 eV is found, but the actual line shape of the alternative fits, and therefore also the dc sheet conductance anisotropy, remains the same.
B. Pb/ Si„335…
The Pb/ Si共335兲system allows the growth of isolated and aligned Pb nanoscale islands, which are sufficiently aniso-tropic to be described as nanowires. Although no RAS mea-surements currently exist for this particular system, the sur-face differential reflection共SDR兲 is known for polarization along, SDRx, and perpendicular to, SDRy, the wire axis.33 The RAS spectrum can be determined from the published SDR data, assuming that the reflectivity of the clean surface is isotropic, RSi,x=RSi,y 共this is a reasonable assumption in the IR regime, well below the SiE1bulk critical point兲.
RSi,x , 共7兲
=2SDRx− SDRy SDRx+ SDRy
In Fig. 6, RAS spectra and SDA, determined from the SDR data of Stròżaket al.33 using Eq.共9兲, are shown for a coverage of 6 ML. A strong RAS signal in the IR is ob-served, accompanied by a sign reversal in the near IR. This is an encouraging sign that, again, the main contribution to the
TABLE I. Free-electron parameters derived by fitting the SDA for various coverages of Sn on InAs共110兲. Parameters which were kept fixed are marked. The confidence interval of the fitted values were below 0.05 eV if not explicitly stated. For 40 ML the region from 1 to 1.5 eV was excluded from the fit because of the strong influence of interband transition in this regime. The last values given are the RAS signal linearly extrapolated to = 0 共兩⌬r/r兩dc,meas兲 and the calculated value for = 0 from the given Drude parameters
共兩⌬r/r兩dc,calc兲. The anisotropic dc sheet conductance was calculated with the fitted Drude parameters using Eq. 共6兲and is given here asd⌬.
Thickness in ML 4 7 14 20 40
d共fixed兲 in nm 0.7 1.3 2.5 3.5 7.2
p共fixed兲 in eV 13 13 13 13 13
␥x in eV 1.5± 0.08 2.1± 0.1 1.30 1.13 1.77
␥y in eV 1.9± 0.08 2.4± 0.1 1.78 1.67 2.02
␥y/␥x 1.26 1.14 1.38 1.48 1.14
兩⌬r/r兩dc,calc 0.02 0.02 0.11 0.21 0.06
兩⌬r/r兩dc,meas 0 0 0.05 0.13 0.08
Re共兩d·⌬兩dc兲 in 10−3S 0.2± 0.05 0.2± 0.05 1.2± 0.2 2.3± 0.5 1.2± 0.4
signal arises from an anisotropic free-electron response and, in particular, an anisotropic scattering rate.
A low surface density of isolated islands is produced at these coverages, with a height much larger than the nominal thickness, in contrast to the simpler case of the tin islands. For example, the island height is explicitly stated to be 13 nm under the particular preparation conditions for a 3 ML sample.33Thusdwas kept as a free parameter, together with
␥y, whilepand␥xwere fixed at the bulk values.26A thick-ness of 6.8 nm was obtained for the 6 ML sample, which is about five times larger than the nominal thickness, but is significantly smaller than the expected island height based on the 3 ML data. The thickness,d, refers to the effective opti-cal layer used to describe the highly percolated system of a few high Pb islands sitting on a metallic wetting layer and hence cannot be directly interpreted as either the average height of the islands or the average thickness of the Pb, in contrast to the much more dense morphology of the Sn islands.
As the spectral region is relatively narrow and only a few data points are available, the parameter values of the aniso-tropic Drude model are less certain than in the case of the Sn islands discussed above: for example, the anisotropic scatter-ing ratio of 10 seems rather high. However, Fig.6shows that the overall line shape can be reasonably reproduced with the anisotropic Drude model. In contrast, the EMA model, using the Pb bulk˜, cannot account for the strong IR signal. By using a larger plasma frequency, the Drude model agreement below 1 eV can be improved, though the discrepancy at the 2 eV data point increases. The experimental value of the anisotropy at 2 eV, derived from the SDR measurements, does not vary much with coverage, which is surprising,
and Pb interband transitions occur in this spectral range, leading to the conclusion that the 2 eV point is unlikely to be determined predominantly by the free electron response. It remains possible that the behavior in the high energy re-gion could arise from percolation effects.36,39 The morphol-ogy of the wires is better known for this system than for Sn/ InAs, but there are insufficient data points to explore this possibility.
Summarizing, a strong infrared RAS signal occurs in two anisotropic metal island systems grown on semiconducting surfaces, with a higher reflectance for light polarized along the long axis of the islands. The signal occurs for both densely packed islands and for isolated wires. The line shape of this signature can be reproduced quite well by a three layer model, where the surface layer is modeled by two in-dependent Drude-like dielectric functions, which allows an anisotropic scattering rate to be introduced, with the lower scattering rate being associated with the long axis of the islands. It thus appears possible to probe anisotropic free electron properties at such surfaces optically, including esti-mating a value of the anisotropy in the dc sheet conductance in favorable cases.
V. ATOMIC NANOWIRES
Quasi-one-dimensional systems, which are much smaller than the island structures discussed so far, can be prepared on surfaces by self-organized growth. Such nanowires may be only four atoms wide and still show metallic properties, as in the case of indium wires on Si共111兲—the Si共111: In-共4 ⫻1兲兲 reconstruction. There are numerous other systems where a metal adsorbate forms one-dimensional structures on a surface, though not all of them show metallic properties: a superficially similar system, Si共111兲: Ag-共3⫻1兲, has a semiconducting surface.40,41
RAS measurements of the Si共111兲: In-共4⫻1兲date back to 1998 and can only be done on the vicinal Si共111兲 surfaces that force single domain formation.13 The RAS spectrum
共Fig. 7兲 is dominated by a strong interband transition at 2 eV. Nevertheless, the measurements show a small but sig-nificant IR anisotropy as well. Possible anisotropic free-electron line shapes arising from the Drude model are shown in Fig.8. In both graphs the thickness of the layer was as-sumed to be d= 1.5 Å, as the metallic surface state is re-ported to be located at the In-Si backbonds;42
p was ap-proximated by the indium surface plasmon frequency. The remaining parameters,␥x= 1.1± 0.2 eV and␥y= 2.8± 0.4 eV, were determined by fitting to the RAS data in the spectral region below 1.2 eV and above 4.5 eV, away from the strong interband transitions.
The fitted␥xscattering rate compares well with the value given from a combined ARPES and conductivity study of 0.8 eV.43 In the same study the sheet conductance of Si共111兲: In-共4⫻1兲 has been measured along, and perpen-dicular to, the chain direction, giving ⌬= 7.1± 0.6 ⫻10−4S /䊐.43 Assuming that the effective thickness of the dc conducting and Drude-type layers are equal, it is then possible, using Eq. 共6兲,44 to calculate the RAS signal at
= 0 as 50± 4⫻10−3. This is ten times larger than the extrapolated value.
FIG. 6. RAS spectra of 6 ML Pb on Si共335兲, determined from the SDR values of Stròżaket al.using Eq.共9兲. The inset shows the corresponding surface dielectric anisotropy. Although only few data points exist, the strong IR signal and a sign change of the RAS can be seen. The former can, in principle, also be explained by an ef-fective medium model 共Bruggeman with ellipsoid inclusions, dashed line兲, but not the latter. The anisotropic free-electron model
共gray line:p= 7.8 eV and␥x= 0.2 eV关bulk values共Ref.26兲兴and
If we include this known dc value as a datum in the fit 共dashed line in Fig. 8兲, the much larger dc anisotropy can be accommodated, and the scattering rates become
␥x= 0.2± 0.04 eV and ␥y= 5.3± 0.8 eV. The shaded area em-phasizes the large change in the shape of the free-electron contribution between these two solutions and shows that, for this system, the dc conductivity cannot be determined reli-ably from RAS measurements above 0.5 eV.
The difficulty in extrapolating, successfully, the measured RAS response in this spectral range to zero frequency arises
from the combination of a small infrared RAS response and strong interband transitions. The small signal cannot be fitted over a sufficiently wide spectral range to produce reliable results, in contrast to the anisotropic island systems dis-cussed above. There are indications that, for Si共111兲: In-共4 ⫻1兲, interband transitions continue to contribute even below 1 eV. Samples with a maximized RAS signal at 1.9 eV usu-ally show a smaller anisotropy at 1 eV共see bars in Fig. 7兲, and the response in this region also changes significantly in the presence of a small excess of In.14,45It is clear from Fig. 8, however, that a small extension of the spectral range to 0.3 eV should allow a much more accurate estimate of the dc sheet conductance anisotropy.
In summary, the amplitude of the infrared RAS response is small for these atomic nanowires, but Fig. 7 shows that metallic and semiconducting structures can be distinguished optically. However, where strong interband transitions are present, it is clear that the spectral range has to be extended further into the IR if the anisotropy in the dc sheet conduc-tance is to be determined, reliably, from the RAS response.
VI. CLEAN METAL SURFACES
Anisotropic surfaces of clean metals should produce an-isotropic electronic properties in the near surface region. Cu共110兲 and Ni共110兲 are two examples of anisotropic sur-faces that have been studied by RAS.27,46,47The RAS spectra of the共1⫻1兲surfaces are shown in the inset of Fig. 9. The RAS spectra of the Ni surface is rather flat, while the Cu spectrum shows a sharp structure at 2 eV, due to a surface state and the onset of d-band transitions. In both cases the
FIG. 7. RAS of the Si共111兲: In-共4⫻1兲 and Si共111兲: Ag-共3⫻1兲 surfaces共black and gray, line respectively兲. The spectra are domi-nated by anisotropic interband transitions around 2 eV. The experi-mental uncertainty of the zero line is indicated by the error bar. The sample-dependent variation of the Si共111兲: In-共4⫻1兲RAS response
共all showing a single domain 4⫻1 LEED pattern兲, is shown at 0.8, 1.9, and 3.8 eV.
FIG. 8. Comparison of the Si共111兲: In-共4⫻1兲RAS signal with the free-electron only response. All model parameters except␥xand ␥y were kept fixed 共see text兲 and only the spectral region below
1.2 eV and above 4.5 eV was included in the fit. For the solid line, only the RAS data were used in the fit, while, for the dashed line, the dc response determined from the measured anisotropy of the sheet conductance 共Ref. 43兲 was included as a zero frequency datum.
FIG. 9. Surface dielectric anisotropy of clean Cu共110兲 and Ni共110兲surfaces. The inset shows the measured RAS spectra for the same surfaces. The SDA shows a strong resemblance to the ex-pected Drude-like dielectric anisotropy for the Ni共110兲 surface
infrared RAS response is quite small. The influence of an anisotropic electron gas has been discussed in the case of the Cu共110兲 surface27 and also for a similar metal surface, Au共110兲,28but in these studies the IR spectral range was not accessible and a free-electron contribution above 1.5 eV was found to be negligible. Figure 9 shows that, in the RAS response共inset兲, no prominent structure arises in the IR, al-though the SDA line shapes, determined from the RAS spec-tra, show the characteristic Drude-like dielectric response. The SDA line shapes can be easily reproduced with the an-isotropic Drude model共see dotted line in Fig.9兲, apart from the interband transitions around 2 and 4.5 eV for Cu共110兲, but there is a significant error associated with fitting these small anisotropies. An erroneous constant RAS signal, C
共zero line offset兲, which can easily occur in a two polarizer configuration, leads to a SDA of C共˜b− 1兲/ 4i, from Eq.
共3兲. Such zero line offsets are typically smaller than ±0.5. The influence of such a systematic error is shown by the shaded area in Fig.9.
Anisotropic roughness, usually modeled by effective me-dia approaches, can also contribute to the dielectric anisotropy.48For anisotropic islands on semiconducting sur-faces, it has been shown above that EMA models, using the bulk metal˜, fail to describe the strong IR structures and the characteristic zero line crossing of the SDA. In the case of metal surfaces, the SDA is smaller and the IR structure is comparable to the metal bulk critical point structures. Hence EMA models can also reproduce the measured SDA. How-ever, for Ni共110兲, the small zero line crossing of the SDA indicates an anisotropic scattering rate contribution to the measured SDA, but morphological anisotropy cannot be completely excluded because the surface roughness, al-though likely to be very small on this single crystal surface, was not quantified.
Summarizing, the measured RAS signal in the accessible IR range from anisotropic metal surfaces is not dominated by a free-electron contribution because normalization by the bulk dielectric function of the metal˜bin Eq.共3兲drastically reduces the measured Drude-like response. The SDA calcu-lated with Eq.共3兲nevertheless does show a Drude-like line shape, which may arise from the near-surface anisotropic electron gas, but other contributions such as surface rough-ness or even systematic errors in the measurement共zero line offset兲 can produce similar signals from the metallic substrate.
VII. LIMITATIONS OF THE APPROACH
It has been shown that, as conventional RAS is extended into the IR region, the anisotropic optical response of metal-lic nanostructures with a strong shape anisotropy, ranging from dense islands to nanowires, becomes significant. It was shown that established anisotropic EMA models, using the bulk response of the metal, cannot describe the response for the samples with the strongest infrared RAS signals. The anisotropic response can be modeled successfully, however, by a surface layer described by two Drude dielec-tric functions. In contrast to the determination of the bulk dielectric functions of metals, where the Drude response can
be easily fitted using two parameters␥ andp, the descrip-tion of the RAS signal needed four independent parameters
共p,␥x,␥y, andd兲—too many for a unique determination of all the parameters. In the examples above, it was possible to fix some of the parameters, typically the thickness of the layer and the plasma frequency, using other data. The model could be extended to include percolation effects by combin-ing an effective medium approach with the anisotropic for-mulation of the free electron gas. Such an extension, involv-ing additional fittinvolv-ing parameters, could not be justified for the spectra discussed here because good agreement was ob-tained with the simpler model, except in regions where the spectra were dominated by interband transitions. For the same reason EMA models used for grid systems,49 which might work well for aligned nanowires, were not explored in detail.
A significant limitation, however, becomes apparent when the IR RAS response is small, as in the case of anisotropic metal surfaces. The output from anisotropic EMA and sur-face layer Drude models may no longer be clearly distin-guishable. It is anticipated that this problem can be alleviated by extending the spectral range further into the IR, where the free-electron-like response will be larger. It has already been shown by Goletti et al. that an extension to 0.3 eV can be achieved with a standard polarizer/PEM setup.50 Conceptu-ally different setups will have to be developed, however, to move further into the IR: one approach would be the use of an FTIR ellipsometer at near normal incidence.
The second limitation concerns the extrapolation of the high frequency conductance anisotropy, as measured by RAS, to obtain the dc sheet conductance, an important pa-rameter for future applications of metallic nanowires. Mea-surements are only possible above 0.5 eV with the current instrumentation, where the anisotropic free electron contribu-tion may be too low, or the interband contribucontribu-tion too high, for reliable fitting. Additionally, the limited spectral range currently available may result in an error in the extrapolated dc value in cases where metallic nanostructures have signifi-cant percolation effects around the experimental cutoff of 0.5 eV.39
The last problem is the limitation of the Drude free electron model itself, which leads to a dielectric function involving a merely phenomenological scattering parameter. However, it is possible to extend the model by allowing for screening 共⬁兲 and by using the effective mass of the electrons m* instead of the free electron mass, an ap-proach used to describe the Drude absorption by free carriers in semiconductors.51Anisotropic parameters are likely to be necessary, however, for modeling the RAS response. Indeed, for Si共111兲: In-共4⫻1兲, it is already known that there is an anisotropy in the effective mass of the electrons and hence the plasma frequency p in the metallic band.52 This more sophisticated model could not be applied because the total number of parameters becomes too large to be useful
showing that the anisotropy in the scattering rate is indeed more dominant 共␥y/␥x between 1.1 and 1.5兲 as was sug-gested in the Introduction. The estimated dc anisotropy var-ies only by 10% and is not particularly sensitive to the details of the model, as the line shape can be reproduced in both cases.
It has been shown that, by extending the spectral range into the IR, it becomes feasible to use RAS as an optical probe of conductance anisotropies in metallic nanostructures. In the case of isolated or dense anisotropic metallic islands on semiconducting substrates, this anisotropic, free-electron-like contribution may even dominate the RAS spectra. If the underlying bulk is also metallic, the anisotropic response of near surface free electrons is less clear and is difficult to
distinguish from anisotropic roughness effects modeled using anisotropic EMAs. For even smaller structures, such as atomic nanowires, the free electron response is small com-pared to anisotropic interband contributions. For these types of systems, extension of the spectral range further into the IR will be necessary to obtain reliable results.
So far only metallic overlayers, which have already been investigated by other techniques, have been studied. As RAS can also probe buried structures, future experiments may be able to reveal if the conductance anisotropy of nanowires is changed when they are covered by protective layers.
The authors would like to acknowledge financial support for this work provided by the Irish Higher Education Authority, IRCSET Grant No. SC/2003/223/, and the SFB 290 of the Deutsche Forschungsgemeinschaft.
*Electronic address: email@example.com
1F. J. Himpsel, K. N. Altmann, R. Bennewitz, J. N. Crain, A.
Kirakosian, J. L. Lin, and J. L. McChesney, J. Phys.: Condens. Matter 13, 11097共2001兲, and references therein.
2H. W. Yeom, S. Takeda, E. Rotenberg, I. Matsuda, K. Horikoshi,
J. Schaefer, C. M. Lee, S. D. Kevan, T. Ohta, T. Nagao, and S. Hasegawa, Phys. Rev. Lett. 82, 4898共1999兲.
3P. Segovia, D. Purdie, M. Hengsberger, and Y. Baer, Nature共
Lon-don兲 402, 504共1999兲.
4M. G. Zacher, E. Arrigoni, W. Hanke, and J. R. Schrieffer, Phys.
Rev. B 57, 6370共1998兲.
5D. E. Aspnes and A. A. Studna, Phys. Rev. Lett. 54, 1956共1985兲.
6V. I. Berkovits, I. V. Makarenko, T. A. Minashvili, and V. I.
Sa-farov, Solid State Commun. 56, 449共1985兲.
7D. E. Aspnes, J. P. Harbison, A. A. Studna, and L. T. Florez, J.
Vac. Sci. Technol. A 6, 1327共1988兲.
8I. Kamiya, D. Aspnes, H. Tanaka, L. Florez, E. Colas, J.
Harbi-son, and R. Bhat, Appl. Surf. Sci. 60–61, 534共1992兲.
9M. A. Herman, W. Richter, and H. Sitter, Epitaxy, No. 62 in
Springer Series in Materials Science 共Sringer-Verlag, Berlin, 2004兲.
10O. Pulci, M. Palummo, M. Marsili, and R. Sole, Adv. Solid State
Phys. 45, 161共2005兲.
11W. G. Schmidt, K. Seino, P. H. Hahn, E. Bechstedt, W. Lu, S.
Wang, and J. Bernholc, Thin Solid Films 455–56, 764共2004兲, and references therein.
12J. R. Power, P. Weightman, and J. D. O’Mahony, Phys. Rev. B
13F. Pedreschi, J. D. O’Mahony, P. Weightman, and J. R. Power,
Appl. Phys. Lett. 73, 2152共1998兲.
14K. Fleischer, S. Chandola, N. Esser, W. Richter, and J. F. McGilp,
Phys. Rev. B 67, 235318共2003兲.
15S. Wang, W. Lu, W. G. Schmidt, and J. Bernholc, Phys. Rev. B
16P. Grosse,Freie Elektronen im Festkörper共Springer, New York
17P. Johnson and R. Christy, Phys. Rev. B 6, 4370共1972兲.
18P. Monachesi, M. Palummo, R. DelSole, R. Ahuja, and O.
Eriks-son, Phys. Rev. B 64, 115421共2001兲.
19J. D. McIntyre and D. E. Aspnes, Surf. Sci. 24, 417共1971兲. 20O. Hunderi, J.-T. Zettler, and K. Haberland, Thin Solid Films
21S. Berthier, J. Phys. I 4, 303共1994兲.
22J.-T. Zettler, J. Rumberg, K. Ploska, K. Stahrenberg, M.
Pris-tovsek, W. Richter, M. Wassermeier, P. Schutzendube, J. Be-hrend, and L. Däweritz, Phys. Status Solidi A 152, 35共1995兲.
23P. K. L. Drude, Ann. Phys. 1, 556共1900兲.
24A. H. Wilson, Proc. R. Soc. London, Ser. A 133, 458共1931兲. 25N. W. Ashcroft and N. D. Mermin,Solid State Physics共Thomson
Learning, Inc., London, 1976兲.
26M. A. Ordal, L. L. Long, R. J. Bell, S. E. Bell, R. R. Bell, J. R. W.
Alexander, and C. A. Ward, Appl. Opt. 22, 1099共1983兲.
27J. Bremer, J.-K. Hansen, and O. Hunderi, Appl. Surf. Sci. 142,
28V. Mazine, Y. Borensztein, L. Cagnon, and P. Allongue, Phys.
Status Solidi A 175, 311共1999兲.
29T. Herrmann, M. Gensch, M. J. G. Lee, A. I. Shkrebtii, N. Esser,
W. Richter, and P. Hofmann, Phys. Rev. B 69, 165406共2004兲.
30The sign in Eq. 共5兲 depends on the sign in the ansatz for the
electromagnetic plane waves. The convention of Ref.19is fol-lowed, withE共t兲= Re关E共兲et兴, leading to˜=⬘−i⬙.
31F. E. Hutchison and W. N. Hansen, Phys. Rev. B 20, 4076共1979兲. 32G. Fahsold, A. Priebe, N. Magg, and A. Pucci, Thin Solid Films
33M. Stróżak, V. Hnatyuk, and M. Jałochowski, Vacuum 74, 241 共2004兲.
34R. A. MacRae and E. T. Arakawa, Phys. Rev. 162, 162共1967兲. 35N. Esser, M. Frisch, A. Röseler, S. Schintke, B. O. Fimland, and
C. Goletti, Phys. Rev. B 67, 125306共2003兲.
36D. Stroud, Phys. Rev. B 19, 1783共1979兲.
37J. Szczyrbowski and K. Schmalzbauer, J. Phys. F: Met. Phys. 16,
38B. Shinozaki, K. Omata, K. Yamada, T. Kawaguti, Y. Fujimori,
39G. Fahsold, M. Sinther, A. Priebe, S. Diez, and A. Pucci, Phys.
Rev. B 70, 115406共2004兲.
40M. Gurnett, J. B. Gustafsson, K. O. Magnusson, S. M. Widstrand,
and S. O. L. Johansson, Phys. Rev. B66, 161101共R兲 共2002兲, and references therein.
41S. Chandola, J. Jacob, K. Fleischer, P. Vogt, W. Richter, and J.
McGilp, J. Phys.: Condens. Matter 18, 6979共2006兲, and refer-ences therein.
42X. López-Lozano, A. Stekolnikov, J. Furthmüller, and F.
Bechst-edt, Surf. Sci. 589, 77共2005兲.
43T. Kanagawa, R. Hobara, I. Matsuda, T. Tanikawa, A. Natori, and
S. Hasegawa, Phys. Rev. Lett. 91, 036805共2003兲.
44Please note that
储from Ref.43corresponds todRe共˜x兲and⬜ todRe共˜y兲 in our notation.
45K. Fleischer, S. Chandola, N. Esser, and J. McGilp, Phys. Status
Solidi B 242, 2655共2005兲.
46J.-K. Hansen, J. Bremer, and O. Hunderi, Phys. Status Solidi A
47D. Martin, S. Barrett, and P. Weightman, J. Phys.: Condens.
Mat-ter 13, 9847共2001兲.
48J. Bremer and O. Hunderi, Phys. Status Solidi A 184, 89共2001兲. 49T. Sergan, M. Lavrentovich, J. Kelly, E. Gardner, and D. Hansen,
J. Opt. Soc. Am. A 19, 1872共2002兲.
50C. Goletti, G. Bussetti, F. Arciprete, P. Chiaradia, and G.
Chiar-otti, Phys. Rev. B 66, 153307共2002兲.
51P. Y. Yu and M. Cardona,Fundamentals of Semiconductors2nd
ed.共Sringer-Verlag, Berlin, 1999兲.